(2) Renewable and Sustainable Energy Reviews 82 (2018) 761–780. Contents lists available at ScienceDirect. Renewable and Sustainable Energy Reviews journal homepage: www.elsevier.com/locate/rser. Advances in reforming and partial oxidation of hydrocarbons for hydrogen production and fuel cell applications. MARK. Sivaprakash Sengodana, Rong Lana, John Humphreysa, Dongwei Dua, Wei Xua, Huanting Wangb, ⁎ Shanwen Taoa,b, a b. School of Engineering, University of Warwick, Coventry CV4 7AL, UK Department of Chemical Engineering, Monash University, Clayton, Victoria 3800, Australia. A R T I C L E I N F O. A B S T R A C T. Keywords: Hydrogen production Catalyst Reforming Partial oxidation Fuel cells. One of the most attractive routes for the production of hydrogen or syngas for use in fuel cell applications is the reforming and partial oxidation of hydrocarbons. The use of hydrocarbons in high temperature fuel cells is achieved through either external or internal reforming. Reforming and partial oxidation catalysis to convert hydrocarbons to hydrogen rich syngas plays an important role in fuel processing technology. The current research in the area of reforming and partial oxidation of methane, methanol and ethanol includes catalysts for reforming and oxidation, methods of catalyst synthesis, and the eﬀective utilization of fuel for both external and internal reforming processes. In this paper the recent progress in these areas of research is reviewed along with the reforming of liquid hydrocarbons, from this an overview of the current best performing catalysts for the reforming and partial oxidizing of hydrocarbons for hydrogen production is summarized.. 1. Introduction. The development of converting hydrocarbon fuels to hydrogen-rich gas products generally fall in one of following processes: steam reforming (SR), auto thermal reforming (ATR), dry reforming (DR), partial oxidation (POX) or a combination of two or more . In spite of their advantages, each of these processes is limited due to factors such as design, fuel and operating temperature. A range of fuel cell systems and common fuel reforming methods have been reviewed by Larminie and Dicks . Thermodynamical analyses of the reforming processes for producing fuel cell feeds of the necessary quality using diﬀerent fuels have been carried out. In 2006, reforming catalysts for hydrogen generation in fuel cell applications was reviewed by Cheekatamarla et al.  There is currently a wide selection of potential fuel reforming catalysts receiving research attention. When investigating a fuel reforming catalyst for fuel cell applications the critical consideration are weight, size, activity, cost, transient operations, versatility to reform diﬀerent fuels/compositions, catalyst durability and fuel processor efﬁciency. A suitable catalyst for fuel reforming will catalyze the reaction at low temperatures, is resistant to coke formation, and is tolerant of diﬀerent concentrations of poisons (e.g. sulphur, halogens, heavy metals, etc.) for an extended period of time. The challenges and opportunities of various fuel reforming technologies for applications in low and high-temperature fuel cells have been previously reviewed [27,29–31]. In previous papers the various steps involved in the generation of fuel cell grade hydrogen with respect to catalyst development. Fuel cells are electrochemical energy conversion devices that are used to convert the chemical energy stored in chemical fuels directly to electrical energy [1–5]. They oﬀer many advantages such as high eﬃciency, low emissions, system compactness and environmental beneﬁts when compared to conventional energy conversion technologies. Among the various types of fuel cells, solid oxide fuel cells (SOFCs) are well recognized due to advantages such as fuel ﬂexibility, high tolerance to impurities in the fuel and not requiring expensive noble metal catalysts [6–14]. In conventional SOFCs, Ni-yttria stabilized zirconia (YSZ) is used as the anode and hydrogen is used as the fuel [15–17]. When this Ni-YSZ anode operated using hydrocarbon fuels instead of hydrogen then an eﬃciency increase can be seen at the system level [18–20]. However, when the Ni-YSZ anode is exposed to hydrocarbon fuels then carbon deposition will occur leading to the system failure [20–22]. When raw fuels, such as diesel, natural gas, and methanol are used, a fuel processor is needed to reform the hydrocarbons into a hydrogen rich gas for the fuel cell to perform the electrochemical conversion [23,24]. This has led to a great interest in converting hydrocarbons into hydrogen. Fuel processing technologies for high temperature fuel cells involve the conversion of hydrogen rich fuels such as gaseous hydrocarbons, gasoline, ammonia, or methanol into a hydrogen rich stream [25,26].. ⁎. Corresponding author at: School of Engineering, University of Warwick, Coventry CV4 7AL, UK. E-mail address: S.Tao.firstname.lastname@example.org (S. Tao).. http://dx.doi.org/10.1016/j.rser.2017.09.071 Received 28 July 2016; Received in revised form 3 July 2017; Accepted 19 September 2017 1364-0321/ © 2017 The Author(s). Published by Elsevier Ltd. This is an open access article under the CC BY license (http://creativecommons.org/licenses/BY/4.0/)..
(3) Renewable and Sustainable Energy Reviews 82 (2018) 761–780. S. Sengodan et al.. has been discussed [32–35]. A couple of excellent reviews on CO2 reforming and partial oxidation of methane are also available [36,37]. The production of hydrogen from steam reforming of ethanol and glycerol was also reviewed in 2005 and 2009 respectively [38,39]. The goal of the present paper is to review and discuss recent progress in the catalyst development, particularly, steam reforming and partial oxidation catalysts and their ability to generate hydrogen from diﬀerent fuel sources for fuel cell applications. The focus will be on transition metals supported on mixed metal oxides and perovskites oxides. This paper surveys four key processes in H2 and syngas production technologies in the following sections, including Section 2 internal reforming for hydrogen production in solid oxide ﬁuel cells, Section 3 – external reforming for hydrogen production (steam reforming of methane, partial oxidation of methane, CO2 Reforming of methane) Section 4 – reforming of liquid hydrocarbons, Section 5 poisoning of catalyst and in Section 6 – reforming and partial oxidation catalysts for direct hydrocarbon solid oxide fuel cells. A summary section is also provided with descriptions on challenges and future work (Section 7), followed by the conclusion section. Some key papers in previous studies are also cited.. Fig. 1. Evolution as a function of time of the anodic gas phase composition compared to the current of the cell; the cell was operated at V = 0.6 V in pure CH4 with a total ﬂow rate of 4 sccm; dashed line represents the levels measured at OCV in diluted H2 at 900 °C .. 2. Internal reforming for hydrogen production Among the various types of fuel cell systems, SOFCs can oﬀer more fuel ﬂexibility by internal reforming of hydrocarbon fuels such as methane, propane, ethanol and natural gas, at the anode [40–42]. Among the various hydrocarbon fuels, methane and propane are the most widely available with vast supply worldwide. By internally reforming hydrocarbon fuels in the SOFCs then an increase in eﬃciency can be observed as well as simplifying the integration of the system. For example, Eric et al. , reported that the eﬃciency of the internal reforming is 8% higher, compared to the external reforming in the same SOFC system. Simpliﬁed thermal management and higher fuel cell performance can be achieved when internally reforming of the fuel is used over external reforming. Also, the internal reforming process in SOFCs can be operated at low steam/carbon ratios compared to the external reforming process. When carrying out internal reforming in a SOFC, it should be noted that the conventional Ni based anode cermet will display poor catalytic activity towards the hydrocarbon and steam/ CO2 reforming due to carbon deposition at the Ni cermet anode. The catalytic modiﬁcation of conventional Ni cermet anode for direct internal reforming is more useful than the identiﬁcation of new anodes which are tolerant to hydrocarbon fuels. In order to improve the reforming reaction of the hydrocarbons while also improving the stability of the Ni cermet anode against carbon deposition a layer of reforming catalyst can be deposited over the Ni anode. Under the direct internal reforming conditions, hydrocarbon fuels with steam/CO2 are passed through the catalytic functional layer, where the fuel is converted into syngas before it reaches the anode. The catalytic layer requires particular properties such as a high catalytic activity towards hydrocarbon reforming and high resistance against carbon deposition. Thus the greater partial reforming reactions occur at the functional catalyst layer with the hydrocarbon fuels converted into syngas as they reach the cermet anode. Zhan et al.  ﬁrst demonstrated the use of Ru-CeO2 catalyst as a direct internal reforming catalyst with the Ni cermet anode. They applied a porous Ru-CeO2 catalyst layer against the Ni cermet anode side of the fuel cell. This porous Ru-CeO2 catalyst layer is used to internally reform the hydrocarbons into syn-gas. Sun et al. studied the eﬀect of morphological features of CeO2 catalyst on direct internal reforming the hydrocarbons . The performance of the fuel cell with mesoporous ﬂower like Ru-CeO2 catalyst shows a power density up to 654 mW cm−2 at 600 °C . Klein et al. studied the Ir (0.1 wt%)-CeO2 catalyst on Ni-YSZ cermet anode in CH4 fuel [46,47]. Fig. 1 shows the anodic gas phase composition compared to current of the cell in pure methane fuel at 900 °C. H2 and CO are the only major products for the internal reforming reaction occurring at the catalyst layer. Fuel cells. with an Ir-CeO2 catalyst show stable fuel cell operation for 120 h in methane at 900 °C and 0.6 V yields a current density of about 100 mA cm−2 . However, it has been noted that the methane concentration gradually increased after 70 h (Fig. 1) indicating that the reforming or partial oxidation activity of the anode started to decrease at this time, however, the fuel cell performance was not aﬀected. One of the possible reasons for this may be due to other mechanisms, such as the direct oxidation of methane playing an important role in retaining the stable current. Wang et al.  studied the eﬀect of Ru loading and their catalytic activities on Al2O3 supported catalysts for internal reforming of methane by partial oxidation, steam reforming and CO2 reforming under SOFC operating conditions. They found that 1 wt% Ru-Al2O3 catalyst shows insuﬃcient catalytic activity towards methane reforming. A 3 wt% RuAl2O3 catalyst shows an outstanding stability and a good thermal stability with the Ni-YSZ anode. Fig. 2 shows the electrochemical performance of 3 wt% Ru-Al2O3 anode in H2, methane-oxygen, methane-steam and methane-CO2 gas mixtures. At 850 °C, the fuel cell using a methaneoxygen mixture shows a peak power density of 1006 mW cm−2, while the same fuel cell shows 1038 mW cm−2 in pure H2. It has been found that addition of metal oxides can improve coke resistance property. Wang et al. [49–51] also studied the eﬀect of promoters Li2O, La2O3, CaO, CeO2, Pr2O3, Sm2O3 and Gd2O3 on the NiAl2O3 catalyst with the aim of improving its coking resistance during fuel cell operation with methane fuels. Among the various promoters, LiLaNi/Al2O3 showed the best catalytic activity and stability compared to LaNi-Al2O3 and LiNi-Al2O3 catalysts. Lee et al.  studied the eﬀect of pore formers in the Ni-Fe anode reforming catalyst on Ni-YSZ fuel cell. The fuel cells containing pore formers (10 wt% carbon black (HB170)) in the Ni-Fe catalyst layer exhibited the highest power density, when compared to the fuel cell containing Ni-Fe catalyst layer without pore formers. It should be noted that some oxides such as CaO, Li2O may react with CO2 to form stable carbonate thereby losing their promoting eﬀects. Liao et al. , studied the doped ceria Ce0.8Zr0.2O2 catalyst for direct internal reforming of ethanol. The high oxygen storage capacity, thermal stability and the ability of doped ceria to promote the water gas shift reaction makes Ce0.8Zr0.2O2 a good catalyst for internal reforming. The catalytic activity is also related to the synthesis process. Liao et al. used diﬀerent synthesis processes to prepare the NiCe0.8Zr0.2O2 catalyst. Ni- Ce0.8Zr0.2O2 catalyst prepared by the glycine nitrate process (GNP) exhibited the best catalytic properties compared to the Ni- Ce0.8Zr0.2O2 catalyst prepared by the inﬁltration method. Above 600 °C, both the Ni- Ce0.8Zr0.2O2 catalysts show a high and 762.
(4) Renewable and Sustainable Energy Reviews 82 (2018) 761–780. S. Sengodan et al.. Fig. 2. I-V and I-P curves of the fuel cells with the 3 wt% Ru-Al2O3 catalyst layer operating on a mixed gas composed of pure hydrogen (a), 80% CH4 and 20% O2 (b), 66.7% CH4 and 33.3% H2O (c) and 66.7% CH4 and 33.3% CO2 (d) at diﬀerent temperatures .. comparable selectivity for H2. However, the catalytic activity decreases signiﬁcantly at low operation temperatures. At 400 °C, the NiCe0.8Zr0.2O2 catalyst prepared by the GNP method shows 70% H2 selectivity, while the inﬁltrated catalyst shows 60.2% selectivity. Ye et al.  also studied the ethanol steam reforming over Cu-CeO2 catalyst. Fuel cells prepared with 21.5 wt% Cu-8.5 wt% CeO2- scandia stabilized zirconia (ScSZ) show power densities of 372 mW cm−2 at 800 °C when C2H5OH + H2O (2:1) was used as the fuel. In addition to stabilized zirconia based and doped cerium oxide based fuel cells, some proton conducting oxides have also been investigated as materials for internal reforming in fuel cells [55,56]. Azimova et al.  studied the BaCe0.48Zr0.4Yb0.1Co0.02O3 perovskite type proton conducting oxides for direct internal reforming of methanol. Fig. 3 shows the electrochemical performance of a methanol/ steam fueled proton conducting SOFC at 600 °C. The fuel cell shows a maximum power density of 65 mW cm−2 in 3:1 (S:C) methanol/water fuel. Jin et al. [57,58], has reported the use of Cu1.3Mn1.7O4 spinel type oxide internal reforming catalyst layer for methane fueled Ni – Sm0.2Ce0.8O1.9 (SDC) SOFC. The fuel cells using the Cu1.3Mn1.7O4 anode catalyst have been shown to exhibit similar electrochemical activities comparable to that of the Ni–SDC anode without a catalyst layer. However, the fuel cells composed of a Cu1.3Mn1.7O4 anode catalyst layer shows a stable performance after 60 h in methane, while the fuel cell without the catalyst layer deactivated quickly in methane. It was found that addition of BaO onto the Ni-based anode can improve the anti-coking property . It was found that nanosized BaO islands grow on the Ni surface, creating numerous nanostructured BaO/ Ni interfaces that readily adsorb water and facilitate water-mediated. Fig. 3. I-V and I-P curves of the Ni- BaCe0.48Zr0.4Yb0.1Co0.02O3 fuel cell anode in 2:1 S:C methanol/water (○) and 3:1 S:C methanol/water (■) fuels at 600 °C .. carbon removal reactions. Besides the metal – metal oxide cermets, some redox stable oxide anode are also used as anode for SOFCs [4,60,61]. At the anode, internal reforming is possible with the presence of H2O and CO2 when hydrocarbon fuels are used in SOFCs. The catalytic activity of these redox stable oxides is very much related to their composition. For example, La0.75Sr0.25Cr0.5Mn0.5O3-δ (LSCM) is a good methane oxidation catalyst while La0.75Sr0.25Cr0.5Fe0.5O3-δ (LSCrF) is an excellent reforming catalyst [10,11]. The use of some 763.
(5) Renewable and Sustainable Energy Reviews 82 (2018) 761–780. S. Sengodan et al.. hierarchically structured NiO/CeO2 nanocatalysts. The template catalyst is fabricated by interwoven ceramic ﬁbers, and the ﬁbers have a nanoporous structure with NiO nanoparticles supported on a CeO2 scaﬀold. Catalyst calcination temperature and its microstructure have a strong inﬂuence on SRM. The catalyst calcined at 950 °C shows the highest performance and stable methane conversion due to its optimized microstructure. Methane conversion was reported about 98% at 800 °C and a steam/CH4 ratio of 2. No catalyst decay was found within 300 min due to the hierarchical microstructure of the nanocatalyst. A number of catalysts based on noble metals such as Ru, Pt, Pd, Ir etc. were tested under methane steam reforming conditions with various supports. Among them, Pd-Rh metal foam (Pd 1.5 wt%, Rh 0.16 wt %, ZrO2 35 wt%, Al2O3 63.7 wt%) has been shown to exhibit good activity and stability in the hydrothermal SRM environment compared to commercial Ru/γ-Al2O3 and Ni/Al2O3 catalysts . At 800 °C the Pd-Rh/metal foam catalyst exhibited steady activity with negligible coke deposition after a stability test of 200 h. For SRM, Ru catalysts have been shown to be very active and selective for H2 production. Simakov et al. , reported that Ru/γ-Al2O3 catalysts with diﬀerent Ru loadings of 0.07, 0.15, 0.30, 1 and 3 wt% can be synthesized by sonication-assisted wet impregnation using ruthenium(III) chloride as a precursor, high surface area aluminum oxide as a support, and acetone as an impregnation medium. Ru/γ-Al2O3 (0.15 wt % loading) catalyst outperforms the commercial (12 wt% Ni-Al2O3) catalyst by two orders of magnitude in terms of methane conversion normalized by metal loading. The minimum limit of the Ru loading is 0.15 wt%, if this limit is lowered; the Ru catalyst activity declines signiﬁcantly which was attributed to the oxidation of sub-nanometer Ru clusters . However, another possibility is that the active site is insuﬃcient to achieve high activity when loading is too low. It was reported that the commercial Ni/α-Al2O3 catalyst was relatively stable at steam to carbon ratio (S/C) = 3 but deactivated rapidly at S/C = 2, losing ca. 70% activity over the course of 15 h  while the Ru/γAl2O3 catalysts is stable even at a low steam to carbon ratio of 1. As shown in Table 1, it is generally diﬃcult to achieve high conversion at a low steam to carbon ratio. The eﬀect of Pd catalysts supported on alumina and mixed with La2O3-Al2O3 oxides was studied by Cassinelli et al. . The authors found that the catalytic performances of Pd catalysts in SRM were signiﬁcantly aﬀected by the type of support. La-containing Pd catalysts exhibit speciﬁc reaction rates in the SRM reaction at 490 °C compared to Pd supported on Al2O3, this is due to the diﬀerent electronic state of Pd. The formation of Pd°[Pdδ+OxLa] species with La support was found to promote the CH4 activation and carbon oxidation. Their results show that the nature of support and the metal–support interface play a very signiﬁcant part in the design of highly active and stable Pd catalysts in SRM. The eﬀect of support material on the surface and catalytic properties of the Pt catalyst when used for SRM were investigated by Rocha et al. . The Pt/La2O3-Al2O3 and Pt/Al2O3 catalyst was obtained by impregnation of the support with an ethanolic solution of H2PtCl6·6H2O. Through extended X-ray absorption ﬁne structure (EXAFS) results it has been shown that the Pt nanoparticles are anchored by weak interaction with the support, the higher stability of Pt catalyst obtained when the La2O3-Al2O3 support was used instead of the Al2O3 is related to the higher thermal stability of Al2O3 modiﬁed with lanthanum. The catalytic activity of Pt supported catalysts for SRM depends on the availability of CH4 to Pt active sites. Yu et al. have prepared Ag-Ni alloy catalysts supported on CeO2 for the reforming reaction of methane and carbon dioxide through the impregnation method . The samples have diﬀerent Ag content with 10 mol% Ni as active sites and 0.3 mol%, 0.6 mol% and 2.4 mol% Ag as the promoter. Table 2 shows the assignments of the ﬁtting components for C1s, Ag 3d, Ni2p3/2 and Ce 3d in X-ray photoelectron spectroscopy (XPS) spectra for Ag promoted Ni/CeO2 catalyst to determine the chemical states and surface compositions. The Ni content at the surface. oxides can prevent the coking on the anode when hydrocarbon fuels are used in SOFCs [60,61]. 3. External reforming for hydrogen production The production of hydrogen rich fuels from hydrocarbons can be achieved through either internal or external steam reforming; from this well established process high eﬃciency for hydrogen production can be achieved. However, the overall steam reforming reaction is endothermic and is generally carried out at the fuel cells high operating temperatures, typically between 500 to 800°C in the presence of a suitable catalyst. The steam reforming reaction can be generalized as follows for hydrocarbon fuels,. Cn Hm + nH2 O → nCO + (n + 1/2m) H2. (1). 3.1. Steam reforming of methane Steam reforming catalysts must meet stringent requirements such as high activity on hydrocarbon conversion, high activity stability, good heat transfer, low pressure drop, high selectivity to hydrogen, high thermal stability and excellent mechanical strength . Steam reforming of methane is a popular method for syngas production and a number of catalysts containing both noble metals and transition metals have been investigated. Catalysts based on Ni have been found to have high catalytic activity and high selectivity for steam reforming of methane (SRM). However, Ni based catalysts also have high carbon coking during SRM. The coking resistance of the Ni catalyst can be improved by the addition of small amounts of noble metals, rare earth metals and supporting materials like perovskites. Since the eﬀects of the additives and support material for the Ni-based catalyst can drastically improve both catalytic performance as well as stability, research in to these areas is very important. The support and additive can be directly involved in the reaction steps facilitating the absorption of the reactant and product formation. Table 1 summarizes the chemical composition of Ni-metal/support catalysts and noble metal/support for steam reforming of methane. Some recently reported examples are brieﬂy discussed. The SRM involves two endothermic reactions (steam reforming) and the exothermic reaction (water gas shift reaction) as follows:. CH4 + H2 O ↔ CO+3H2. ΔH°298 K = 206.1 kJ mol−1. (2). CO + H2 O ↔ CO2 + H2. ΔH°298 K = −41.1 kJ mol−1. (3). CH4+2H2 O ↔ CO2+4H2. ΔH°298 K = 165.1 kJ mol−1. (4). When Ni-metal/support is used as the SRM catalyst, we have to pay close attention to preparation methods in order to ensure that a high catalytic activity is achieved for the modiﬁed catalysts. A typical catalyst synthesis method is the impregnation method using an aqueous solution containing Ni. When Ni/SiO2 catalyst was prepared by impregnation method followed by dielectric barrier discharge (DBD) it shows an advantage of having smaller particle sizes, leading to a moderate methane decomposition rate and a better balance between carbon depositions. Besides, the catalyst prepared conventionally by calcination shows a much larger particle size . In a recent work, Zhang et al.  studied SRM over Ni based core shell catalyst Ni/Al2O3 – silicalite zeolite by diﬀerent synthesis methods. The catalyst consists of a Ni/Al2O3 core and silicalite zeolite shell. Their main ﬁnding shows that an inactive NiAl2O4 spinel phase was formed during repeated calcination at elevated temperatures. Among the catalysts tested the catalytic activity of the core shell catalyst for the SRM reaction displayed a 10% improvement over catalysts prepared by traditional method. Cerium oxide was used as a support material for nickel catalysts and the eﬀect of SRM at a temperature of 800 °C was investigated by Wang et al. . A template synthesis process has been adopted to prepare 764.
(6) Renewable and Sustainable Energy Reviews 82 (2018) 761–780. S. Sengodan et al.. Table 1 Chemical composition of Ni-metal/support catalyst and noble metal/support for steam reforming of methane. Catalyst. Preparation method. Temperature (°C). Weight hour space velocity (ml h−1 gcat−1). Steam to carbon ratio (S/C). Conversion (%). H2 selectivity (%). Ref.. Ni/La2Zr2O7. Coprecipitation/ impregnation impregnation impregnation impregnation. 800. 18,000. 2. 100. > 75. . 600 655 700. 2700 n/a 471,000. 4 3 3. 86 88 100. 92 75.   . impregnation impregnation impregnation impregnation impregnation impregnation Precipitation/ impregnation impregnation Stöber process/ deposition precipitation impregnation co-precipitation. 800 650 600 500 800 550 700 600 750. 24,000 96,000 9600 2000 6000 3000 24,000 105,000 6600. 0.5 1 4 3 3 4 4 0.5 3. 40 77.2 80 > 85 32.2 84 85 > 30 85. NA 68.3 NA > 97 NA NA 55 NA 45.         . 650 700. 42,000 210,000. 2.5 2. 82 > 85. NA NA.  . urea hydrolysis/ impregnation hydrolysis EDTA-citrate method/ impregnation. 800. 54,000,000. 2. 98.6. NA. . 700 700. 560,000 25,500. 3 2. 75 85. NA NA.  . 600 800. 60,000 30,000. 1 1. 45 85. 35 NA.  . 600. 15,000. 3. 80. NA. . 700. 20,000. 4. > 95. > 72 NA NA NA NA 81 NA 68. . Ni-nano-CaO/Al2O3 Ni/γ-Al2O3 Ni–Pt/ Al2O3 anodic alumina support Ni/SiO2 Pt-Ni/Al2O3 Ni-Pt/MgAl2O4 Ni-Cu/Al2O3 Ni-Rh/Al2O3 Ni-Au/Al2O3 Mo/Ni/Al2O3 Ag-Ni/Al2O3 Ni@SiO2 Ni/MgSiO3 M/Ni0.5/Mg2.5(Al)O M= Rh, Pt, Pd M/Ce0.15Zr0.85O2 M=Pt, Ru, Rh Ni/Ce1−xGdxO2 Ni/ CeO2-HfO2 Ni/CaO–ZrO2-Al2O3 Ru/NixMg6−xAl2. Ru/MgO-Nb2O5. Hydrotalcite process/ impregnation hydrotalcite route/ impregnation impregnation. Rh/CeO2. impregnation. 800. 40,000. 1.2. 99.4. Rh/xSm2O3-yCeO2-Al2O3 Zr0.95Ru0.05O2−δ LaNiO3 Ru/γ-Al2O3. sol–gel/ impregnation sonochemical method spray pyrolysis sonication-assisted wet impregnation. 760 650 777 600. 6,480,000 61,800 300,000 750. 3 1 1 1. 70 74 75 75. Ru/Co6−xMgxAl2.     . formation and modiﬁes the coke from whisker carbon or graphitic carbon to amorphous carbon. SRM on the Sn/Ni/YSZ catalyst was reported by Nikolla et al. through a combination of kinetic studies, isotopic-labeling experiments, and DFT calculations [94–96]. Fig. 4 shows the kinetic isotope studies on Ni/YSZ and Sn/Ni/YSZ catalyst surface with labeled methane CD4 . They reported that kinetic isotope eﬀects are similar in degree by the rate of C–H bond dissociation on both catalysts. From this kinetic we are able to draw conclusions about the mechanisms accountable for the improved carbon-tolerance of Sn/Ni compared to Ni. Sn atoms are reasonable for the rate-controlling CH4 activation step to move from low-coordinated Ni sites to the well-coordinated Ni-Sn sites. Sn preferentially displaces the Ni atoms from the under-coordinated sites. In presence of the Sn, the activation barrier for the dissociation of CH4 is. of Ni/CeO2 is estimated to be higher than that in the bulk, indicating a surface enrichment of Ni on the Ni/CeO2. For 0.3 mol% Ag Ni/CeO2 and 2.4 mol% Ag Ni/CeO2, the surface contents for Ni are still higher than that of the bulk surface, showing Ag does not aﬀect the Ni content enrichment at the catalyst surface. Generally, as Ag and Ni form surface alloys on the Ni surface, the Ag content should be higher than that in the bulk in the XPS measurement. The diﬀerence came from fact that partially reduced CeO2 can migrate onto the Ni surface and bury Ni particles into the catalyst support. The CeO2 migration causes the Ni enrichment at the Ag-Ni/CeO2 surface. The catalyst with 0.3 mol% Ag loading subjected to a stability test was shown to be resistant to coke deposition. 0.3 mol% Ag decreases the intrinsic activity of Ni surfaces and concurrently increases the long term (100 h) stability under various feedstock conditions. Also, the Ag promoter decreases the coke. Table 2 Assignments of the ﬁtting components for C1s, Ag 3d, Ni2p3/2 and Ce 3d in XPS spectra of catalyst . Catalysts Ni/CeO2. Ni/CeO2–0.3Ag. Ni/CeO2–2.4Ag. C 1s Ni3C Graphite CO32− Ni3C Graphite CO32− Ni3C Graphite CO32−. Content (at%) 0.00% 83.03% 16.97% 0.63% 90.81% 8.56% 7.93% 65.89% 26.17%. Ag 3d. Content (at%). Ni 2p3/2. Content (at%). Ce 3d 4+. Content. Ni° Ni2+. 27.26% 72.74%. Ce Ce3+. 83.45% 16.55%. Ag Agn+. 74.05% 25.95%. Ni° Ni2+. 21.98% 78.02%. Ce4+ Ce3+. 74.35% 25.65%. Ag Agn+. 86.63% 13.37%. Ni° Ni2+. 6.40% 93.60%. Ce4+ Ce3+. 59.44% 40.56%. 765.
(7) Renewable and Sustainable Energy Reviews 82 (2018) 761–780. S. Sengodan et al.. Fig. 4. The rate of steam reforming is measured for CH4 and CD4 reactants as a function of time on (a) Ni/YSZ at 700 °C and (b) Sn/Ni/YSZ at 760 °C. The dark lines depict points in time when the reactant is switched from CH4 to CD4 and back to CH4. The steam-to-carbon ratio was 1 .. increased while also decreasing the binding of the carbon atoms to the low-coordinated sites. This will thereby inhibit the nucleation of carbon at Ni sites. In other words, the Sn alloying with Ni atoms preferentially oxidize C atoms from C–C bonds and/or decreasing the thermodynamic driving force for carbon nucleation on Ni sites. A Cu promoted Ni/Al2O3 was prepared and studied by Khzouz et al.  in order to improve the SRM and suppress the carbon deposition. The activity of Cu-Ni/Al2O3 was compared with that of commercial Ni/ Al2O3, Cu/ZnO/Al2O3 catalysts. Morphological characterization results showed that the average particle size increases when compared to the commercial Ni/Al2O3 catalyst. The prepared Cu-Ni/Al2O3 catalyst exhibited low selectivity for CO and it was shown to be more selective to H2 in methane. Fig. 5 shows the SRM for Cu-Ni/Al2O3 and the commercial Ni/Al2O3 catalyst. The Cu-Ni/Al2O3 catalyst showed a methane fuel conversion of 98% with 99% hydrogen selectivity at 650 °C. The improved performance of Cu-Ni/Al2O3 catalyst can be due to the formation of a Ni–Cu alloy which could be formed. This Ni-Cu alloy may be responsible for blocking and decreasing the number of sites involved in the carbon formation.. MgO and Nb2O5 have both been employed as the additives for SRM in the Ni/Al2O3 catalyst. MgO as a support increases the CO2 selectivity of the process at a steam to carbon (S/C) molar ratio of 2, Nb2O5 is well known for its acidic nature. Both MgO and Nb2O5 provide strong metal–support interaction. Amjad et al.,  reported the use of MgO and Nb2O5 as the support for the Ru catalyst. Ru was introduced to the MgO and Nb2O5 support by the wet impregnation method before calcining at diﬀerent temperatures. The Ru/ Nb2O5 catalyst shows higher activity in terms of CH4 conversion, CO2 selectivity, and H2 dry outlet concentration compared to MgO supported catalyst. The prepared catalyst showed diﬀerent Ru oxidation states in XPS spectra depending on the preparation condition and precursor used. Homsi et al.  studied the combination of MgO and Al2O3 supported Ru catalysts (CoxMg6−xAl2) for SRM. The basic nature of MgO allows it to resist coking due to the enhancement in the oxidation rate of CHx fragments which are adsorbed on the Ru active metal. The acidic nature of Al2O3 will facilitate the decomposition of methane. Four diﬀerent CoxMg6−xAl2 (x = 0, 2, 4 and 6) supports were prepared by the hydrotalcite route and Ru was introduced to the CoxMg6−xAl2 support by wet impregnation method, this was then calcined at 500 °C. Fig. 6 shows the X-ray diﬀraction (XRD) spectra of Ru-CoxMg6−xAl2 catalyst calcined in air at 500 °C. The supports with a high Mg content showed more intense RuO2 diﬀraction lines with increased RuO2 particle size. In the presence of high Co loading RuO2 leads to the formation of smaller particles that are well dispersed on the Co6Al2 support making it non detectable by the XRD technique. At high Co loadings Ru interacts diﬀerently from that obtained with the Mg rich support. The SRM on Ru/Co6Al2 catalyst showed the highest H2 molar concentration produced as well as the lowest CO concentration, demonstrating that Ru/Co6Al2 catalyst favors the water gas shift (WGS) reaction. The improved reactivity of high cobalt content catalyst is due to the result of improved surface properties of the support. An opposite behavior was. Fig. 5. Methane steam reforming over a) Ni–Cu/Al2O3 catalyst and b) Ni/Al2O3 catalyst .. Fig. 6. XRD patterns (“s”: Co3O4/CoAl2O4/Co2AlO4; “○”: MgAl2O4; “∼”: MgO; “∗”: RuO2; “+”:Co2RuO4) .. 766.
(8) Renewable and Sustainable Energy Reviews 82 (2018) 761–780. S. Sengodan et al.. Fig. 7. H2 fraction obtained using LCFN-0.2 (•) and commercial catalyst (★) for various S/C ratios at 700 °C .. observed for the Mg rich support as well as an intermediate behavior observed for Ru/Co4Mg2Al2 and Ru/Co2Mg4Al2 catalysts. Additionally, the Ru/Co6Al2 catalyst is stable for 100 h on stream. Various transition materials like Ni, Co, Fe and noble metals like Pt, Rh, Pd, Ir, and Ru have been reported to be active for SRM. However, deactivation of the catalyst due to carbon deposition was a major problem. Perovskite oxides (ABO3) have been studied as catalysts for the production of syngas from hydrocarbon fuels. Perovskite oxides generally contain rare-earth elements in A-site (like La, Sr, or Ba) which determines the thermal stability of the catalyst and B site is occupied by a 3d transition metal, such as Ni, Co, or Fe, which determines the catalytic activity for steam reforming. Perovskite-type oxides are widely studied due to their high stability under a wide range of oxygen partial pressures as well as their ability to form metallic particles in the order of the nanometers under reforming condition which diminish coke formation. Choi et al.  studied the SRM over La1−xCexFe0.7Ni0.3O3 (x = 0.1 ≤ x ≤ 0.5) perovskite catalysts and compared their results with a commercial catalyst containing 10–14 wt% of NiO and 86–90 wt % of Al2O3. Fig. 7 shows the H2 produced with La0.8Ce0.2Fe0.7Ni0.3O3 (LCFN-0.2) and a commercial catalyst at 700 °C with diﬀerent S/C ratios. The H2 produced using the commercial catalyst decreased from 79% to 51.9% when the S/C ratio was decreased from 3 to 1, while the H2 produced using LCFN-0.2 catalyst remain unaﬀected with the S/C ratio. The amount of coke formed on the commercial catalysts was 48.7 wt% and 0.2 wt% for LCFN-0.2 after a 20 h stability test. In the perovskite LCFN catalyst, lattice oxygen vacancies in the perovskite structure may be responsible for enhanced coke gasiﬁcation of the carbon species formed over the catalyst. The oxygen vacancies also act as active sites for the dissociation of steam under the reaction condition. Urasaki et al.  studied the SRM on Ni catalyst supported on a variety of perovskite oxides, including LaAlO3, LaFeO3, SrTiO3, BaTiO3, La0.4Ba0.6Co0.2Fe0.8O3−δ (LBCF), and compared the catalytic activity and resistance to coking of perovskite catalysts to the conventional Ni/ Al2O3 catalyst. Perovskite catalysts LaAlO3, LaFeO3, LBCF were prepared by the Pechini method and the catalysts were calcined at 850 °C for 11 h. SrTiO3 and BaTiO3 catalyst were prepared by solid state reaction at 1150 °C for 10 h. 10 wt% Ni was introduced in the perovskite catalyst by impregnation using an aqueous solution of Ni(NO3)2·6H2O. Fig. 8 shows the activities of various Ni/perovskite catalysts and the conventional Ni/Al2O3 catalyst in SRM tested at 800 °C with a steam to methane ratio of 2. The catalytic activity of Ni/LaAlO3 and Ni/SrTiO3 catalyst were comparable to that of the conventional Ni/Al2O3 catalyst. Meanwhile, the catalytic activity of Ni/LaFeO3 showed a lower activity while the activities of Ni/BaTiO3 and Ni/LBCF were also extremely poor. The Ni/LaAlO3 and Ni/SrTiO3 catalyst showed CH4 conversion levels of 91.7% and 88.4% after being run for 1 h, respectively. Temperature programed reduction (TPR) studies showed that a larger amount of lattice oxygen is removed from Ni/BaTiO3 during reduction. Fig. 8. Catalytic activities of supported Ni catalysts. Catalyst; (○) Ni/LaAlO3, (■) Ni/ SrTiO3, (•) Ni/LaFeO3, (▴) Ni/BaTiO3, (▾) Ni/LBCF, (♢) Ni/Al2O3. Reaction conditions: temperature, 800 °C; molar H2O/CH4 ratio, 2 .. with hydrogen when compared with either the Ni/LaAlO3 or Ni/SrTiO3 catalyst. This explains why the Ni/LaAlO3 and Ni/SrTiO3 catalysts displayed higher catalytic activities than Ni/BaTiO3, because LaAlO3 and SrTiO3 catalysts have a larger amount of lattice oxygen near the surface and metallic nickel. The lattice oxygen present close to active nickel sites can be easily transferred to CHx fragments adsorbed on metallic nickel, which facilitates the oxidation of CHx fragments. Therefore, transition element based perovskite oxides are promising anti-coking catalysts for the reforming of hydrocarbons. It should be noted that there is a process which combines steamreforming of methane and CO2 absorption together in a single reaction step over a steam reforming catalyst mixed with a CO2 absorbent. This process is called sorption-enhanced H2 production. The removal of the produced CO2 from the system by the solid absorbent makes reaction (4) shift to the right thus methane conversion will be enhanced. The produced H2 can have a purity of 98% with only a small amount (ppm level) of CO and CO2 thus minimizing the requirement on puriﬁcation. However, the CO2 absorbent may be saturated after a period of time thus regeneration is required which can be achieved through temperature or/and pressure swing. The sorption-enhanced H2 production has been covered by a few excellent reviews [100–105]. The key challenge is the multicycle durability of CO2 absorbent which must be improved . Hydrogen production through chemical looping was also investigated. In 1993, Steinfeld and Kuhn proposed to production hydrogen through combining methane and solar thermal with the use of Fe produced from Fe3O4 as the reaction catalyst . First, methane reacts with Fe3O4 to form Fe, H2 and CO according to the following reaction,. Fe3 O4 + 4CH4 = 3Fe + 8H2 + 4CO. (5). The molar ratio of produced CO and H2 is 1:2 which can be used as an important intermediate for the gasto-liquids (GTL) process for the production of liquid hydrocarbons . In the following step, steam is introduced to the system to react with the produced Fe, forming pure H2,. 4H2 O + 3Fe = Fe3 O4 + 8H2. (6). The advantage of this chemical-looping H2 production is that a gas separation process is not required. The produced pure H2 and syngas in the individual step are both very useful chemical products. Chemical 767.
(9) Renewable and Sustainable Energy Reviews 82 (2018) 761–780. S. Sengodan et al.. Table 3 Chemical composition of Ni-metal/support catalyst and noble metal/support for partial oxidation of methane. Catalyst. Preparation method. Temperature (°C). Weight hour space velocity (ml h−1 gcat−1). O2 to carbon ratio (O/C). Conversion (%). H2 selectivity (%). Ref.. M/Mg/Al M = Rh, Ni, Rh/Ni, Ir/Ni or Ru/Ni Pt/Ni/Al2O3 Pt M + Ni/Al2O3 M = Ru, Rh, Pd, Pt Pt-NiO/Al2O3 M/Ni/Al2O3 M = Ru, Pd, Pt Co/Al2O3 Pt–Co/Al2O3 Ni/ 12CaO·7Al2O3. co-precipitation. 750. 339,292. 0.5. 92. 40. . impregnation impregnation. 800 800. 225,000 90,000. 0.5 0.5. 85 > 80. NA > 90.  . impregnation Precipitation/ impregnation impregnation impregnation solid-state reaction/ impregnation solid-state reaction/ impregnation impregnation impregnation impregnation impregnation impregnation impregnation hydrothermal/ impregnation impregnation impregnation impregnation impregnation impregnation combustion/ impregnation impregnation impregnation combustion impregnation combustion/ impregnation hydrothermal coprecipitation coprecipitation Sol-gel/ impregnation Stober method Precipitation/ impregnation impregnation impregnation Pechiney impregnation impregnation. 800 800. 7200 560,000. 0.5 0.5. 91.8 > 80. 98.4 90.  . 850 750 800. 60,000 56,000 30,000. 0.5 0.4 0.5. 95 95 > 90. 93.6 NA > 95.   . 800. 30,000. 0.5. > 90. > 90. . 800 850 800 800 800 850 700. 144,000 20,000 60,000 60,000 62,000 62,000 5000. 0.5 0.5 0.5 0.5 0.55 0.55 0. 90 95 100 97.4 95 95.5 NA. > 95 98.1 96.6 95 98.5 > 40.       . 850 800 750 850 700 800. 27,000 152,432 110,000 270,000 195,000 28,500. 0.5 0.5 0.5 0.5 0.5 0.5. 97 80.3 94.3 > 90 85 > 60. NA NA 98 > 95 NA NA.      . 600 800 700 750 750. 88,500 500,000 480,000 3,000,000 532,121. 0.5 0.55 0.5 0.5 0.38. 80 88.1 > 80 > 90 > 30. 97.5 NA NA NA.     . 700 750 750 750 750 750. 60,000 354,044 111,357 20,000 50,000 50,000. 0.5 0.5 0.5 0.5 0.5 0.5. 95.2 93 90 > 75 > 90 > 85. 92.9 95 > 95 > 95 > 75 > 65.      . 750 800 750 800 700. 90,000 60,000 12,000 4800 30,000. 0.5 0.5 0.5 0.5 0.5. 100 > 90 > 80 86.3 > 70. NA.     . Sol-gel combustion solid-state reaction hydrothermal Pechiney Sol-gel Pechiney combustion. 600 800 915 900 900 850 950 700 900. 50,400 899,550 20,000 66,000 30,000 30,000 73,600 72,000 848. 0.5 0.25 0.48 0.5 0.5 0.5 0.13 0.5 0.51. > 75 > 35 > 75 > 94 > 50 > 70 94 83.9 > 80. 85.9 > 70.         . solid-state reaction solid-state reaction. 900 777. 5940 22,400. 0.5 0.5. 89 83. NA 95.  . Pt/12CaO·7Al2O3 Ni-Co/CaAl2O4/Al2O3 Co/MgO Co/ZrO2 Co/La2O3 NiCoMgCeOx/ZrO2-HfO2 NiCoMgOx/ZrO2-HfO2 NiCo/SBA–15 LiNiLaOx//Al2O3 Ni/CeO2/Al2O3 NiO/La2O3/γ-Al2O3 LiLaNiO/Al203 Ni–Cr/Al2O3 NiFe-ZrO2/Cu Ir-Ni/Al2O3 Pt-Ni/Al203 Ni–Pt/La0.2Zr0.4Ce0.4Ox Pt/Ni0.5/MgAlOx Cu-Ni/Ce0.9Zr0.1O2 Rh-CeO2 Ni-Rh/Al2O3–MgO Rh/Ni/Mg/Al hydrotalcite Ni/SiC Ni/ZrO2@SiO2 core shell Ni/CeO2 Ni/zeolite catalysts Ni/CeO2–La2O3 Ni/CeO2-Al2O3 Ni/TiO2 Ni-M/Anodic TiO2 M=Ru, Pt, Rh NiO-Al2O3 LaCoO3/γ-Al2O3 NdCaCoO3.96 Sr0.8Ni0.2ZrO3 La0.08Sr0.92Fe0.20Ti0.80O3 La0.5Sr0.5CoO3 Gd0.33Ba0.67FeO3 Ni@SiO2 core shell La0.3Sr0.7Fe0.7Cu0.2Mo0.1O3 membrane reactor La2NiO4 membrane reactor Yb2Ru207. > 90 99.7 > 70 > 75 > 40 > 90 NA > 60 > 75. oxygen carriers for the chemical looping steam methane reforming to syngas and hydrogen co-production . Another strategy to prevent sintering and improve the stability of the catalyst has been the introduction of pores into the oxygen carrier. It has been reported that macroporous CeO2-ZrO2 solid solutions are excellent oxygen carrier for chemical-looping stream reforming of methane . Both sorption-enhancement and chemical looping H2 production are very attractive due to gas separation being minimized or not required at all, however, there are challenges that must be overcome before any real applications can be achieved.. looping H2 production has been reviewed by Tang et al.  There are some key reports in chemical-looping production of hydrogen using Fe2O3-CeO2 as the oxygen carrier [107,109,110]. The key challenge is carbon deposition when the oxide reacts with methane therefore making reaction (5) incomplete. Sintering of the formed Fe is another problem . The weak oxidation ability of H2O leading to a low oxidation degree and slow oxidation rate also remain as challenges . It is therefore very important to ﬁnd suitable oxygen carriers which have a good reactivity and high agglomeration resistance for this process. It was found that perovskite oxides LaFe1−xCoxO3 are good 768.
(10) Renewable and Sustainable Energy Reviews 82 (2018) 761–780. S. Sengodan et al.. 3.2. Partial oxidation of methane for hydrogen production Partial oxidation, in which methane, natural gas or a hydrocarbon is heated in the presence of a stoichiometric amount of pure oxygen, has attracted a lot of attention in recent years. Partial oxidation of methane shows several advantages over steam reforming including; good response time, compactness, and less sensitivity for fuel variation. Partial oxidation reactors are gaining increased interest in the energy conversion ﬁeld particularly in high temperature fuel cells. Partial oxidation of methane is a highly exothermic reaction and is considered as a faster reaction than the SRM .. Cn Hm +. 1 m nO2 → nCO + H2 2 2. Fig. 9. Schematic representation of Ni/CeO2 and CeO2 surface having surface defects with under coordinated oxygen atoms .. (7) based catalyst materials exhibited good catalytic activity, good stability and the ability to restrain itself from carbon deposition. It has been claimed that the perovskite catalyst can be used to bring down the threshold value needed to generate the carbon deposition. Carbon deposition can also be prevented through the reaction of the oxygen species over the perovskite reacting with the carbon deposition. Staniforth reported a Sr0.8Ni0.2ZrO3 perovskite catalyst with high selectivity and activity for POM . Fig. 10 shows the stability of this Sr0.8Ni0.2ZrO3 perovskite catalyst for diﬀerent cycles at a temperature of 900 °C. Catalyst deactivation was not observed during the stability test with a high stability of the Sr0.8Ni0.2ZrO3 perovskite catalyst shown for the reducing environment at 900 °C. A similar result was also reported by Meng et al. when using a LaGa0.65Mg0.15Ni0.20O3 (LGMN) perovskite catalyst for the partial oxidation of methane to syngas . The LGMN perovskite catalyst syngas selectivity reached up to 100% with the methane conversion reaching values larger than 81% at 900 °C. Post analysis test on the catalyst after POM showed that the LGMN catalysts contain a major perovskite phase and other phases like La2O3, La2O2CO3 along with metallic Ni.. The partial oxidation of hydrocarbon to syn-gas (CO + H2) can occur at very high temperatures without the use of a catalyst; however, the operating temperature will be signiﬁcantly reduced with the use of catalysts. Partial oxidation of methane (POM) to fuel rich syn-gas can be represented as,. CH4 +. 1 O2 → CO + 2H2 2. ΔH°298 K = −35.6 kJ mol−1. (8). The most studied catalysts for POM are similar to steam reforming catalysts including supported transition metals (Ni, Co, and Fe), noble metals and perovskite oxides . Although, transition metals are active catalyst components for POM, the metal species with diﬀerent oxidation states plays a signiﬁcant role in the methane conversion steps. When referring to a Ni supported catalyst, metallic nickel is used to promote the formation of syn-gas, and the Ni species with oxidation number ≥2 will promote the total combustion of methane. In general, the distribution of the catalyst metallic species with various oxidation states depends on the synthesis process and the support properties. Table 3 summarizes the diﬀerent catalyst systems investigated in the literature. In the reported catalysts, Co/ZrO2 is an excellent low cost catalyst with both high conversion and H2 selectivity . Pantaleo et al.  studied the POM of a Ni catalyst supported over CeO2, La2O3 and mixed CeO2-La2O3. The Ni catalyst supports were prepared by co-precipitation and wet impregnation. During stability tests it was observed that carbon formed only on the single oxide supported catalysts, Ni/CeO2 and Ni/La2O3. In the presence of mixed supports like CeO2-La2O3 carbon did not formed, this was due to the formation of diﬀerent nickel–lanthanum oxide species with diﬀerent Ni oxidation states. It was also reported that the defect species over the support play an important role in the POM by Pal et al. . Fig. 9 shows the schematic representation of Ni/CeO2 and CeO2 surface showing surface defects with under coordinated oxygen atoms. When the Ni content is low (i.e., up to 2.5% Ni) in CeO2, the defects are mainly substitution defects. The enhancement of the interstitial and surface (structural) defects by the formation of the –O-Ni-O-Ce super structure with exposure to highly under-coordinated O atoms can be achieved by further increasing the Ni content in CeO2. These undercoordinated O atoms strongly interact with the C–H bond facilitating the cleavage of weakened C–H bonds, while the pure CeO2 shows a lower aﬃnity of CH4 toward the “Ce center”, due to absence of point defect and surface defects. Abbasi et al. studied the monolith supported noble metal (Pt, Pt:Pd, and Pd) catalyst for POM . The results of the POM test showed that the most active catalyst for both wet and dry feeds was Pd, which was followed in order of decreasing activity by Pt:Pd and then by Pt. Santis-Alvarez et al. investigated the eﬀect of diﬀerent supports (Al2O3 and Ce0.5Zr0.5O2) on a Rh based catalyst . It was found that Rh oxidation was inhibited by the Al2O3 support and POM over Rh/ Ce0.5Zr0.5O2 catalyst support was limited due to continuous re-oxidation of metallic Rh by oxygen spillover from the support. Among studied catalysts for POM, it was found that perovskite. 3.3. CO2 reforming of methane for hydrogen production Dry reforming of methane (DRM) with CO2 is very attractive in terms of syngas production as it can be used to convert greenhouse gases (CH4 and CO2) into valuable fuel rich syngas for both domestic and industrial utilization. In the dry reforming process carbon dioxide is used to reform methane to obtain syngas (H2 and CO) by the following reaction:. CH4 + CO2 → 2H2+2CO. ΔH°298 K = 247 kJ mol−1. (9). In reality the above reaction proceeds through a number of complex intermediate steps involving absorption, disproportionation, recombination and desorption. These intermediate reactions typically. Fig. 10. Methane conversion during reaction of methane and limited oxygen (CH4:O2 = 2) over Sr0.8Ni0.2ZrO3 for diﬀerent cycles at a reaction temperature of 900 °C .. 769.
(11) Renewable and Sustainable Energy Reviews 82 (2018) 761–780. S. Sengodan et al.. Table 4 Chemical composition of metal/support catalyst used for dry reforming of methane. Catalyst. Temperature (°C). Weight hour space velocity (ml h−1 gcat−1). CO2 to carbon ratio (CO2/C). Conversion CH4 (%). Conversion CO2 (%). H2/CO ratio. Ref.. 2% Cr–40% Ni/CeO2 Ni-Pt/Al2O3 5%Ni/Ce0.8Pr0.2O2 Ni/SBA–15 Ir/Ce0.9Pr0.1O2 Ni/CeO2-TiO2 Ni-Al2O3 Ni-Mo2C/La2O3 Ni@SiO2 Ni-Ce/MgAl2O4 Ni17W3 alloy/ SiO2 Co-Ce/ZrO2 Co/CeO2 NiMgxAly NiPtx/Al2O3 Co-Zr/Activated Carbon Pt/PrO2–Al2O3 Rh/CaO-SiO2 4% Ni–0.2% Au 0.2% Pt–10% CeO2 Ni/CeAlO3-Al2O3 NiO-MgO-ZrO2 La1−xSrxCoO3 LaNixFe1−xO3 Ni-Ce0.8Zr0.2O2 La0.9Ba0.1NiO3 Rh-CeO2 Ni-Ba/Al2O3 Ru/Ce0.75Zr0.25O2 Rh-Ni/ Boron Nitride MxLa1−xNi0.3Al0.7O3 M=Li, Na,K La0.95Ce0.05NiO3 LaNi1−xMgxO3 LaNi0.8Ru0.2O3 Ce2Zr1.51Ni0.49Rh0.03O8 LaNi0.95Rh0.05O3 Pt -Ni/nanoﬁbrous-Al2O3 Rh/Al2O3. 850 700 750 650 750 800 800 800 750 700 800 700 750 800 700 750 650 650 800. 10,200 7500 30,000 52,800 18,000 14,400 72,000 12,000 40,000 10,000 96,000 20,000 30,000 80,000 20,000 7200 48,000 222,222 60,000. 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1. 90 65 71.5 98 61.1 > 80 > 85 60 71.2 > 90 60 > 70 79.5 80 87.2 90.6 67.3 11.8 93.41. 95 76 83.4 86 74.5. 97.26. NA 0.65 1.20 1.09 0.97 0.73–0.82 NA NA 0.75 NA NA > 0.6 NA NA 0.96 NA 0.84 0.53 NA.                   . 800 750 800 800 750 700 750 700 900 700 750 750 700 750 800 650 700 800. 20,000 64,500 24,000 300,000 44,800 24,000 11,100 30,000 12,000 60,000 15,000 72,000 600,000 72,000 12,000 40,000 30,000 60,000. 1 0.67 1 1 0.92 1 1 1 1 1 1 1 1 1 1 1 1 1. 80 65 93.6 80 73.2 50 48.6 60 96 72 90 50 57 80 30 70 > 65 56.9. 90 75 98.9 NA 85 55 57 70 98 81 NA 60 67 85 100 NA > 70 NA. NA NA NA 0.95 NA 0.66 0.73 0.6 1 0.7 1 0.4 0.47 0.6 NA NA NA NA.                  . 2CO ↔ C+CO2. ΔH°298 K = −171 kJ mol−1. inﬂuence the DRM reaction by the reverse water gas shift (RWGS) reaction, which leads to a H2/CO ratio diﬀerent from less than unity.. CO2 + H2 ↔ CO + H2 O. ΔH°298 K = 41.2 kJ mol−1. ΔH°298 K = 75 kJ mol−1. (12). Therefore to reduce coke deposition in the DRM reaction the use of a catalyst system that eﬀectively reduces this is required. The use of Ni and Co based catalysts is a preferable choice due to their abundance, high activity and the economically feasible cost. However, the Ni catalyst suffers from rapid deactivation and coke formation. Diﬀerent type catalysts such as, Ni, Ru, Rh, Pd, Ire, Pt or Co, on a oxide support, such as SiO2, Al2O3, MgO, TiO2, CaO, CeO2, ZrO2, or La2O3 have been studied for DRM in order to overcome the coke formation . Table 4 summarizes the chemical composition of metal/support catalysts and noble metal/supports for DRM. Among the investigated, Ni/SBA-15 is a promising one with high CH4 and CO2 conversion plus high H2 to CO ratio .. (10). In addition to the diﬃculties associated with the RWGS reaction DRM has the inherent disadvantage of rapid catalyst deactivation due to carbon buildup on the catalyst surface. Coke deposition can be either formed by methane decomposition and/or by CO disproportionation reaction (Boudouard reaction) to form solid carbon on the catalyst surface producing H2.. CH4→C+2H2. > 85 80 58.4 > 90 70 NA 87.6 95 90 88.5 79.2. (11). Fig. 11. Stability test for Ni@SiO2 with 3.3 nm and 11.2 nm shell thickness. Conditions: 800 °C, GHSV = 36,000 ml g–1 cat h–1, CO2:CH4:N2 = 1:1:1 .. 770.
(12) Renewable and Sustainable Energy Reviews 82 (2018) 761–780. S. Sengodan et al.. Fig. 12. CH4 and CO2 conversion eﬃciency as a function of temperature (700–850 °C) for various Nibased Al2O3 catalysts (Ni/Al2O3, NiCoMg/Al2O3, and WNiCoMg/Al2O3), (b) long-term stability of CH4 and CO2 conversion of catalysts up to 3000 h at 850 °C (Reaction conditions: P = 1 atm, CH4:CO2:N2 = 1.0:1.0:1.0, GHSV = 80,000 h−1) .. Eﬀective stabilization of the metal catalyst against coke formation can be achieved through percolating the metal catalyst with inorganic layers such as SiO2 and Al2O3. A new Ni@SiO2 core shell catalyst introduced by Zhang et al. to study the DRM shows a stable performance by reducing the formation of coke on the catalyst surface . Similarly, Li et al. studied the eﬀect of shell thickness with Ni@SiO2 catalyst towards DRM . It was found that a small increase in the shell thickness of the Ni@SiO2 catalyst results in dramatic improvements in catalyst stability and speciﬁc activity towards CH4 and CO2. Fig. 11 shows the stability test for Ni@SiO2 with 3.3 nm and 11.2 nm shell thickness at 800 °C. The high catalytic activity of Ni@SiO2 was due to the eﬀective void space between the Ni core and the SiO2 shell providing a uniform reaction environment which improves the adsorption ability of Ni towards methane. Addition of basic metal oxide supports to the DRM (eg: MgO) catalyst provide a promising alternative to minimize carbon deposition. The basicity of these supports and/or promoters will bring a more favorable CO2 adsorption through the formation of bicarbonate (HCO3-) or carbonate species (CO32-) were the CO2 interacts with basic OH surface species or O2− surface ions. Son et al. reported a high carbon resistant MgO promoted NiCo/Al2O3 catalyst (WNiCoMg/Al2O3) with a MgAl2O4 nano island decorated on the DRM catalyst . Fig. 12 shows the performance of Ni/Al2O3, NiCoMg/Al2O3, and WNiCoMg/ Al2O3 catalyst at atmospheric pressure using high gas hourly space velocity (GHSV) of 80,000 h−1 showing an excellent stability over 3000 h. The excellent catalytic activity and long term stability of WNiCoMg/Al2O3 catalyst mainly originates from the robust structure of the catalyst itself.. Fig. 13. Representation of intermediate species molecular structures of ethanol steam reforming on catalyst surfaces.. Fig. 14. Representation of intermediate species molecular structures of methanol steam reforming on catalyst surfaces.. 4. Reforming of liquid hydrocarbons for hydrogen production. 4.1. Reforming of methanol for H2 production. The production of hydrogen from liquid hydrocarbons such as ethanol, methanol, etc. has received considerable research attention due to their economic importance and environmental beneﬁts [204,205]. Unlike SRM, steam reforming of liquid hydrocarbons involves complex pathways and intermediate products which depend on the nature of the metal surface. For example ethanol steam reforming (ESR), commonly reported surface intermediated species  such as acetaldehyde (CH3CHO*), acetyl (CH3C*O), ketene (*CH2C*O), and ketenyl (*CHC*O) and other intermediate species like *CHyCHx*OH and *CH2CH2O* are formed on the metal catalyst surface. Their molecular structures are shown in Fig. 13. Similarly, the commonly identiﬁed surface intermediate species  formed during methanol steam reforming (MSR) are methoxy (*OCH3), formaldehyde (*OCH2), dioxymethylene (*OCH2O*), mono-dental formate (*OCHO), bidental formate (*OCHO*), and methyl formate (*OCHOCH3). Their molecular structure is shown in Fig. 14. Table 5 summarizes the chemical composition of the Ni-metal/support catalyst and noble metal/support for steam reforming of liquid hydrocarbons. Among the investigated catalysts, Cu-based catalysts are the best in terms of cost and conversion.. Experimental studies of MSR carried out on Ni-Cu/ZrO2 catalyst have been reported by Lytkina et al.  using diﬀerent Ni and Cu ratios and annealing temperatures. ZrO2 was prepared by the precipitation method and the resulting samples were sequentially impregnated with aqueous solution of Cu and Ni. The obtained bi-metallic catalysts were further annealed at 350 and 400 °C followed by reduction at 350 °C in H2. Four catalyst supports prepared with diﬀerent Cu/ Ni ratios and at diﬀerent temperatures were produced. (1). Cu0.8-Ni0.2/ ZrO2 350 °C; 2) Cu0.2-Ni0.8/ZrO2 400 °C; 3) Cu0.8-Ni0.2/ZrO2 400 °C; 4) Cu0.2-Ni0.8/ZrO2 350 °C. Thermal analysis (DSC) and XRD patterns shows that the catalyst annealed at 350 °C is amorphous whereas the catalyst annealed at 400 °C has a monoclinic structure. For all compositions of the catalyst support a methanol conversation was archived at over 350 °C. Fig. 15 shows the temperature dependence of hydrogen formation on diﬀerent Ni-Cu/ZrO2 catalysts. The catalyst annealed at 350 °C (amorphous) shows higher hydrogen production compared to catalyst annealed at 400 °C (monoclinic). It is well known that water absorption on the catalyst surface plays an important role in reforming reactions. The increase in H2 production on the Cu0.8-Ni0.2/ZrO2 350 °C 771.
(13) Renewable and Sustainable Energy Reviews 82 (2018) 761–780. S. Sengodan et al.. Table 5 Chemical composition of Ni-metal/support catalyst and noble metal/support for steam reforming of liquid hydrocarbon. Catalyst. Fuel. Preparation method. Temperature (°C). Weight hour space velocity (ml h−1 gcat−1). Steam to carbon ratio (S/C). Conversion (%). H2 selectivity (%). Ref.. CuNi/CeO2 Cu/ZnO CuZnZrAl Cu–Mn spinel Cu/ZnO Cu/ZnO/ZrO2/Al2O3 ZnO/Cu/SiO2 CuO/ZnO/CeO2/ZrO2/Al2O3 Cu/ZnO/ZrO2/Al2O3 Cu–Zn–Ce–Al-oxide Ce1−xCuxO2 CuxMn3−xO4 spinel Ni/La2O3-ZrO2 Ni/CeO2-ZrO2 Ni/GDC Ni/TiO2 Ni0.95Mo0.05/SBA CuNi/SiO2 PtNi/CeO2 Pt1.5Cox/ZrO2 Ni3Mg2AlOY Co2MnO4 2KCo/ZrO2 La0.6Sr0.4CoO3 La1−xCaxFe0.7Ni0.3O3 La1−xKxFe0.7Ni0.3O3 LaCoxNi1−xO3 Ni/LaFe0.7Co0.3O3 Mn/Co10Si90MCM Rh/La2O3(5%)CeO2–Al2O3 Rh/CeO2 Ir/CeO2 Ir/CeO2 Ir/Ce0.9Pr0.1O2 Rh-Co/CeO2 Rh/MgO Pt/CeO2 Pt/CeZrO2. ethanol methanol methanol methanol methanol methanol methanol methanol methanol methanol methanol methanol ethanol ethanol ethanol ethanol ethanol ethanol ethanol ethanol bio ethanol ethanol ethanol ethanol ethanol ethanol ethanol ethanol ethanol ethanol ethanol ethanol ethanol ethanol ethanol ethanol bio ethanol ethanol. impregnation homogeneous precipitation impregnation soft reactive grinding soft reactive grinding precipitation hydrolysis/ polymerization precipitation precipitation impregnation precipitation combustion impregnation impregnation hydrothermal/ impregnation precipitation/ impregnation hydrothermal impregnation hydrothermal/ impregnation sol-gel/impregnation. 450 250 350 260 300 260 300 270 300 260 260 280 350 650 850 500 700 350 500 300 300 700 420 700 650 450 550 550 600 500 650 650 450 450 450 650 350 500. 57,000 12,600 903 10,080 7680 60,000 21,200 22,909 276,000 7331 5000 14,008 9180 5517 80,000 29,160 8571 17,177 36,000 22,000 168,000 8571 60,000 40,000 400,000 60,000 60,000 80,000 8571 82,200 381,703 6000 22,000 18,000 72,000 24,000 25,350 80,000. 10 1.2 1.4 1.3 1.3 1.3 1.5 1.1 1.3 1.4 1 1.5 30 8 3 3 3 6 3 13 3 0.33 9 3 3 3 3 3 0.33 3 3 1.8 4 3 3 8.4 3 0. 60 100 > 50 92.9 100 > 90 > 75 90.5 100 90 90.7 100 100 100 100 99.5 80 100 69 100 100 100 100 100 100 100 100 100 100 70 100 100 100 95 90 100 82 100. 70 NA.                                      . combustion impregnation sol–gel citrate pechini method pechini method pechini method pechini hydrothermal/ impregnation impregnation deposition-precipitation deposition–precipitation deposition–precipitation impregnation impregnation impregnation impregnation precipitation/ impregnation. 99.5 60 NA NA NA NA. 94.3 55 > 75 65 NA 80 NA NA 60 71 74 70 65 70 60 67 97 70 72 55 NA 60 60 92 > 50. shown in Fig. 16. The catalytic performance of Ni-Mo2C has a strong dependence on the methanol conversion. When the Ni loading is low (Ni/Mo = 0.8/99.2–2.4/97.6) the catalyst exhibits the highest methanol conversion with a reaction temperature of 300 °C, when the Ni molar ratio increases to over 5 the methanol conversion decreases sharply. The XRD and BET results shows that the Ni particles loaded on the Mo2C were sintered together and covered the surface of molybdenum carbide at a high Ni/Mo ratio (5/95, 10/90, and 15/85), which results in the decrease in the methanol conversion. The superior catalytic activity of lower Ni/Mo (0.8/99.2–2.4/97.6) is due to the synergistic eﬀect between Ni and native Mo2C which plays a prominent role in the methanol conversion. Fig. 16b shows the stability of β-Mo2C, Fe-Mo2C (1.6), Co-Mo2C (1.6), and Ni-Mo2C (1.6) catalysts for the MSR reactions at 400 °C. The Ni-Mo2C (1.6) showed a comparatively longer catalytic stability and the higher methanol conversion for 12 h. XPS studies show that Mo2+ species on fresh and spent β-Mo2C decreases from 40% to 8% due to surface oxidation. The high performance and stability of Ni modiﬁed Mo2C may be due to a higher resistance to oxidation than pure molybdenum carbide and Fe-, Co modiﬁed carbides catalyst. LaCoO3-based perovskite oxides have also been studied for several oxidation and reduction reactions. Recently, La–Sr–Co–FeO perovskite mixed oxides have attracted considerable attention due to their high mixed electronic-ionic conduction properties and a good catalytic activity towards methane oxidation, as well as their chemical stability in the reducing conditions. Kuc et al. studied the eﬀect of Pd and Zn substation on the LaCo1−x−yPdxZnyO3 ± δ perovskite catalyst for. Fig. 15. Temperature dependence of H2 yields in MSR on obtained catalysts .. catalyst may likely be due to the signiﬁcantly higher content of water molecules absorbed on the surface of amorphous ZrO2 catalyst than monoclinic ZrO2 catalyst. Besides oxides, carbides have also been investigated as the catalyst supports for reforming of liquid hydrocarbons Ma et al. studied the catalytic activity of metal modiﬁed Mo2C catalysts for MSR with different M/Mo molar ratios . The catalyst were prepared by mixing aqueous solutions of (NH4)6Mo7O24·4H2O, Ni(NO3)2·6H2O, Fe (NO3)3·9H2O and Co(NO3)2·6H2O, respectively and calcining at 500 °C. Carburization of M–MoO3 to M-Mo2C was carried out in a ﬁxed-bed quartz microreactor with a CH4/H2 (20 vol% CH4) atmosphere. The MRS of Ni-Mo2C with diﬀerent doping amount of Ni (Ni/Mo ratio = 0.8/99.2, 1.2/98.8, 1.6/98.4, 2.4/97.6, 5/95, 10/90, and 15/85) was 772.
(14) Renewable and Sustainable Energy Reviews 82 (2018) 761–780. S. Sengodan et al.. comparative study of ESR on two series of catalysts: (i) Ni deposited on CeO2 or La2O3 promoted alumina; and (ii) Ni deposited on CeO2 or La2O3 promoted zirconia were reported by Dan et al. . The catalysts were prepared through the impregnation method on Al2O3 and ZrO2 supports with an aqueous solution of Ce and La followed by calcining. The mixed supports contain 6 wt% CeO2 and 6 wt% La2O3. Finally Ni (8 wt%) was introduced on the CeO2-Al2O3, La2O3-Al2O3, CeO2-ZrO2, and La2O3-ZrO2 supports, followed by calcination in argon at 550 °C and reduction in H2 at 550 °C. Fig. 18 shows the catalytic activity of the Ni supported, CeO2 and La2O3 promoted, Al2O3, and ZrO2 catalysts for ESR at temperatures between 150–350 °C. For both the Al2O3, and ZrO2 catalysts promoted with La2O3, 100% ethanol conversion was reported at 300 °C. Also, the ESR was improved by addition of CeO2 on the ZrO2 supported catalyst, addition of CeO2 on Al2O3 was not signiﬁcant on the ethanol conversion. High H2 yield was observed by coupling the Rh/CeO2 catalyst on ESR at 400 °C, this was due to the remarkable C–C bond breaking capacity of the Rh catalyst . CeO2 support was prepared by the urea precipitation process and was then calcined in air at 400 °C. 1% Rh loaded catalyst was further prepared by a deposition-precipitation method. Fig. 19 shows the ESR over the Rh/CeO2 catalyst. At 400 °C, ethanol and other intermediate products like acetone, acetaldehydes were not detected, suggesting that ethanol was entirely converted into hydrogen and other C1 products (CO, CO2, CH4). At high temperature (650 °C), the reformed gas contains 72 mol% H2, 14 mol% CO, 10 mol% CO2 and 4 mol% CH4. For the Ni on perovskite supports, Ni/BZCYYb (BaZr0.1Ce0.7Y0.1Yb0.1O3), Ni/BZCY7 (BaZr0.1Ce0.7Y0.2O3) and Ni/ BZCY4 (BaZr0.4Ce0.4Y0.2O3) a higher catalytic activity and lower carbon deposition than other oxide catalysts was observed [222,226]. Ex situ Raman spectroscopy was performed to investigate carbon formed on the catalyst (Fig. 20). Without the addition of steam in the feed, Ni/ BZCYYb and Ni/BZCY7 display comparable graphitization. When the steam content is increased in the feed, the carbon deposition was much lower in the Ni/BZCYYb catalyst than in the Ni/BZCY7 catalyst. It was reported that the high carbon tolerance of BaZrO3-BaCeO3 oxides is due to the water storage capability, the addition of Yb eﬀectively improves the catalytic activity for the ethanol steam reforming reactions. The stored water in the proton-conducting oxide may react with deposited carbon forming relevant gases thus carbon deposition was alleviated.. Fig. 16. (a) Catalytic performances of Ni-modiﬁed molybdenum carbide with diﬀerent doping amounts. (b) Stability of β-Mo2C, Fe-Mo2C (1.6), Co-Mo2C (1.6), and Ni-Mo2C (1.6) catalysts for the SRM reaction at 400 °C .. MSR . A series of LaCoO3 ± δ (LCO), LaCo0.873Pd0.127O3 ± δ (LCPO), LaCo0.89Zn0.11O3 ± δ (LCZO), LaCo0.95Pd0.025Zn0.025O3 ± δ (LCPZO-5), LaCo0.85Pd0.075Zn0.075O3 ± δ (LCPZO-15), and LaCo0.75Pd0.125Zn0.125O3 ± δ (LCPZO-25) perovskite oxides were prepared by the Pechini method and calcined at 800 °C in air. The methanol conversion and CO2 selectivity were studied for all the perovskite compositions. It was observed that Pd and Zn containing LCPZO-5, LCPZO-15 and LCPZO-25 show superior CO2 selectivity in the 200–400 °C temperature range than the un-substituted or mono substituted materials LCO, LCPO and LCZO. For example, at 225 °C, the CO2 selectivity is around 11% on un-substituted LCO, on the other hand, for substituted it is between 70% and 91% over Pd and Zn containing perovskite materials. The CO2 selectivity was shown to improve with increasing Pd and Zn content in LCPZO-5 and LCPZO-15. Fig. 17 shows the 1st derivative of the mass loss curves (DTG) of the perovskite catalyst materials. From Fig. 17b it is evident that the positions of lowtemperature DTG curves shifts progressively to lower temperatures with increasing Pd (and Zn) content in the due to the increased reducibility with the presence of the Pd substituent, the materials with both Pd and Zn (LCPZO) leading to signiﬁcantly improve the MSR activity (≥ 80% CO2 selectivity).. 5. Poisoning of catalysts for reforming and partial oxidation of hydrocarbons The stability of catalysts for reforming and partial oxidation of hydrocarbons is extremely important. The deactivation and regeneration of catalysts may be caused by various reasons including chemical, thermal and mechanical which have been reviewed by Argyle et al. . The recent progress beyond this excellent review is brieﬂy described below. Poisoning by impurities, mainly sulphur is the major challenge for reforming and partial oxidation catalysts, whilecoking also poses a problem for reforming catalysts, particularly at low oxygen partial pressure. Recently Ocsachoque et al. reported that the Rh/CeO2 catalyst exhibits a higher tolerance to sulphur than the Ni/CeO2 catalyst, this is because of the existence of O2- species in the former. The O2- species can help to oxidize sulphur into SOx . As for the conventional Ni/Al2O3 catalyst, it was found that a high sintering temperature is beneﬁcial to the anti-coking property when performing the CO2 reforming of methane. NiAl2O4 will be formed at high temperature while Ni particles formed from the reduction of NiAl2O4 have a strong interaction with the support while carbon deposition did not aﬀect the contact of gases with the supported Ni catalysts thus the activity remains . Not only methane, reforming of dodecane and liqueﬁed petroleum gas has attracted the attention of researchers. It was found that LaNiO3 nanocrystals in SBA-15 mesoporous SiO2 exhibits high stability and anti-coking on steam reforming of liqueﬁed petroleum .. 4.2. Reforming of ethanol for H2 production For ethanol steam reforming Rh [211,212] and Ni  based catalysts are the most commonly studied with a very high selective towards hydrogen production. The studied supports were Al2O3 [214,215], MgO [216,217], ZrO2 , CeO2 , La2O3 , Nb2O5 , perovskites [221,222] and bi-metallic [223,224]. A 773.
(15) Renewable and Sustainable Energy Reviews 82 (2018) 761–780. S. Sengodan et al.. Fig. 17. 1st derivative of the mass loss (DTG) curves of (a) LCO ( ) and LCZO ( ) and (b) LCPZO-5 ( ( ( ) and LCPZO-25 ( ) .. 2000, Gorte et al. extended the hydrocarbon fuels for SOFCs from methane to ethane, 1-butene, n-butane and toluene . The development of anodes for hydrocarbon SOFCs have been reviewed in several papers [61,262,266,267]. Reformed liquid hydrocarbons such as ndodecane and diesel are also reported as fuels for SOFCs with good performance although the degradation is slightly higher than that when H2 was used as the fuel [268–270]. MoO2 has been identiﬁed as a conductive anti-coking anode running on reformed diesel. There is also some initial work on the reforming of diesel/biodiesel to be used as fuels for SOFCs . Conventional Ni-based anodes for SOFCs suﬀer from carbon deposition due to Ni being an excellent hydrocarbon decomposition catalyst. While this can be avoided to a large extent by having excess water in the system to promote steam reforming reactions, this requirement can increase system complexity and add water management issues. The ability to utilise the fuel directly with less or no additional water would be a great beneﬁt for system by reducing the cost, thus a good reforming catalyst that can work at low steam to carbon ratios would be ideal. This can be realised whether as part of direct utilization on the anode itself or as part of a robust pre-reforming catalyst supplying partly reformed fuel to the anode. It has been reported that when Ni is replaced by Cu, Cu alloys, or with the integration of CeO2, carbon deposition can be alleviated [265,272]. Liu reported that BaO-Ni/YSZ anode can run C3H8 as the fuel exhibiting stable performance for 100 h . The ﬁrst redox perovskite-based anode (La0.75Sr0.25)Cr0.5Mn0.5O3δ (LSCM) was discovered by Tao and Irvine. This can run on methane as the fuel with negligible carbon deposition . Other material families such as titanate , vanadate [61,274] and double perovskite  are also reported to be redox stable/reversible and with promising performances when run on hydrocarbon fuels [61,267]. Besides these requirements, carbon deposition, tolerance to impurities (particularly sulphur), long term operational reliability and durability remain challenges, especially when liquid hydrocarbons such as diesel/bio-diesel are used as the fuel. Therefore some element of pre-reforming is essential in these cases . For gaseous hydrocarbons, reforming of the fuels will generate H2 and CO to be used as the fuels for SOFCs however, care must still be exercised to prevent reverse water gas shift reactions resulting in the formation of solid carbon. Anti-coking can also be achieved through tailoring of microstructure. It has been reported that hierarchically porous Ni-based anode deposited with a nanocatalyst layer has improved coking resistance when methane was used as the fuel. A thin layer of nano samaria doped ceria catalyst was inﬁltrated on the walls of Ni-yttria-stabilised zirconia anode. The cell eﬃciency has been improved with a power density of 650 mW cm−2 at 800 °C when methane was used as the fuel while the performance is stable for over 400 h. This study provides an excellent strategy in developing anticoking anodes for SOFCs . In addition to carbon deposition and poisoning, sintering of catalysts is a further key challenge in order to realise a stable robust anode for SOFCs. In general, oxidation of hydrogen is easier than that for CO and hydrocarbons. An anode with integrated reforming or oxidation catalysts for in situ hydrogen. ), LCPO ), LCPZO-15. 6. Reforming and partial oxidation catalysts for direct hydrocarbon solid oxide fuel cells The high fuel ﬂexibility oﬀered by SOFCs gives the possibility to use relatively cheap, safe, and readily available hydrocarbons. However more direct utilization of such fuels would greatly lower fuel cost and increase the feasibility of SOFC commercialization, especially for nearterm adoption in high value markets. This also allows the technology to create a bridge towards the anticipated arrival of the “hydrogen economy”. Current SOFC technology has shown good performance with a wide range of hydrocarbon and syngas fuels, but there are still signiﬁcant challenges for practical application . The direct utilization of hydrocarbons in an SOFC was reported by Vohs et al. as early as 1995 but the power density was not high . In 1999, Barnett et al. reported a direct methane SOFC without carbon deposition when a 0.5 µm thick (Y2O3)0.15(CeO2)0.85(YDC) porous ﬁlm was used between the Ni-Y2O3-stabilized ZrO2 (YSZ) anode and YSZ electrolyte . In. Fig. 18. The variation of ethanol conversion with temperature in ethanol steam reforming reactions catalyzed by: (a) alumina supported Ni catalysts and (b) zirconia supported Ni catalysts; 1 g catalyst, 0.1 ml/ min liquid ﬂow, 35 ml/min Ar ﬂow .. 774.